General

Property | Temperature | Value |
---|---|---|

Density | 20.0 °C | 7.85 g/cm³ Show Material materials with Density of 7.85 g/cm³ |

Mechanical

Property | Temperature | Value |
---|---|---|

Elastic modulus | -100.0 °C | 217 GPa Show Material materials with Elastic modulus of 217 GPa |

20.0 °C | 212 GPa Show Material materials with Elastic modulus of 212 GPa | |

100.0 °C | 207 GPa Show Material materials with Elastic modulus of 207 GPa | |

200.0 °C | 199 GPa Show Material materials with Elastic modulus of 199 GPa | |

300.0 °C | 192 GPa Show Material materials with Elastic modulus of 192 GPa | |

400.0 °C | 184 GPa Show Material materials with Elastic modulus of 184 GPa | |

500.0 °C | 175 GPa Show Material materials with Elastic modulus of 175 GPa | |

600.0 °C | 164 GPa Show Material materials with Elastic modulus of 164 GPa | |

Elongation | 20.0 °C | 25 % Show Material materials with Elongation of 25 % |

Poisson's ratio | 20.0 °C | 0.28 [-] Show Material materials with Poisson's ratio of 0.28 [-] |

Tensile strength | 20.0 °C | 340 - 490 MPa Show Material materials with Tensile strength of 340 - 490 MPa |

Yield strength | 20.0 °C | 215 - 235 MPa Show Material materials with Yield strength of 215 - 235 MPa |

Yield strength Rp0.2 | 100.0 °C | 186 MPa Show Material materials with Yield strength Rp0.2 of 186 MPa |

200.0 °C | 157 MPa Show Material materials with Yield strength Rp0.2 of 157 MPa | |

250.0 °C | 147 MPa Show Material materials with Yield strength Rp0.2 of 147 MPa | |

300.0 °C | 118 MPa Show Material materials with Yield strength Rp0.2 of 118 MPa | |

Unlock all property charts |

Thermal

Property | Temperature | Value |
---|---|---|

Coefficient of thermal expansion | -100.0 °C | 1.08E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.08E-5 1/K |

20.0 °C | 1.19E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.19E-5 1/K | |

100.0 °C | 1.25E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.25E-5 1/K | |

200.0 °C | 1.3E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.3E-5 1/K | |

300.0 °C | 1.36E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.36E-5 1/K | |

400.0 °C | 1.41E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.41E-5 1/K | |

500.0 °C | 1.45E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.45E-5 1/K | |

600.0 °C | 1.49E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.49E-5 1/K | |

Unlock all property charts | ||

Specific heat capacity | -100.0 °C | 423 J/(kg·K) Show Material materials with Specific heat capacity of 423 J/(kg·K) |

20.0 °C | 461 J/(kg·K) Show Material materials with Specific heat capacity of 461 J/(kg·K) | |

100.0 °C | 479 J/(kg·K) Show Material materials with Specific heat capacity of 479 J/(kg·K) | |

200.0 °C | 499 J/(kg·K) Show Material materials with Specific heat capacity of 499 J/(kg·K) | |

300.0 °C | 517 J/(kg·K) Show Material materials with Specific heat capacity of 517 J/(kg·K) | |

400.0 °C | 536 J/(kg·K) Show Material materials with Specific heat capacity of 536 J/(kg·K) | |

500.0 °C | 558 J/(kg·K) Show Material materials with Specific heat capacity of 558 J/(kg·K) | |

600.0 °C | 587 J/(kg·K) Show Material materials with Specific heat capacity of 587 J/(kg·K) | |

Unlock all property charts | ||

Thermal conductivity | 20.0 °C | 56.9 W/(m·K) Show Material materials with Thermal conductivity of 56.9 W/(m·K) |

100.0 °C | 56.4 W/(m·K) Show Material materials with Thermal conductivity of 56.4 W/(m·K) | |

200.0 °C | 53.5 W/(m·K) Show Material materials with Thermal conductivity of 53.5 W/(m·K) | |

300.0 °C | 49.4 W/(m·K) Show Material materials with Thermal conductivity of 49.4 W/(m·K) | |

400.0 °C | 45.2 W/(m·K) Show Material materials with Thermal conductivity of 45.2 W/(m·K) | |

500.0 °C | 41.3 W/(m·K) Show Material materials with Thermal conductivity of 41.3 W/(m·K) | |

600.0 °C | 37.6 W/(m·K) Show Material materials with Thermal conductivity of 37.6 W/(m·K) | |

Unlock all property charts | ||

Thermal diffusivity | 20.0 °C | 15.7 mm²/s Show Material materials with Thermal diffusivity of 15.7 mm²/s |

100.0 °C | 14.5 mm²/s Show Material materials with Thermal diffusivity of 14.5 mm²/s | |

200.0 °C | 12.9 mm²/s Show Material materials with Thermal diffusivity of 12.9 mm²/s | |

300.0 °C | 11.2 mm²/s Show Material materials with Thermal diffusivity of 11.2 mm²/s | |

400.0 °C | 9.6 mm²/s Show Material materials with Thermal diffusivity of 9.6 mm²/s | |

500.0 °C | 7.9 mm²/s Show Material materials with Thermal diffusivity of 7.9 mm²/s | |

600.0 °C | 6.3 mm²/s Show Material materials with Thermal diffusivity of 6.3 mm²/s | |

Unlock all property charts |

Electrical

Property | Temperature | Value |
---|---|---|

Electrical resistivity | 20.0 °C | 1.83E-7 Ω·m Show Material materials with Electrical resistivity of 1.83E-7 Ω·m |

100.0 °C | 2.27E-7 Ω·m Show Material materials with Electrical resistivity of 2.27E-7 Ω·m | |

200.0 °C | 2.95E-7 Ω·m Show Material materials with Electrical resistivity of 2.95E-7 Ω·m | |

300.0 °C | 3.8E-7 Ω·m Show Material materials with Electrical resistivity of 3.8E-7 Ω·m | |

400.0 °C | 4.81E-7 Ω·m Show Material materials with Electrical resistivity of 4.81E-7 Ω·m | |

500.0 °C | 5.99E-7 Ω·m Show Material materials with Electrical resistivity of 5.99E-7 Ω·m | |

600.0 °C | 7.38E-7 Ω·m Show Material materials with Electrical resistivity of 7.38E-7 Ω·m | |

Unlock all property charts |

Chemical properties

Property | Value |
---|---|

Carbon | 0.13 % Show Material materials with Carbon of 0.13 % |

Chromium | 0.5 - 0.8 % Show Material materials with Chromium of 0.5 - 0.8 % |

Copper | 0.3 - 0.5 % Show Material materials with Copper of 0.3 - 0.5 % |

Manganese | 0.2 - 0.5 % Show Material materials with Manganese of 0.2 - 0.5 % |

Nitrogen | 9E-3 % Show Material materials with Nitrogen of 9E-3 % |

Phosphorus | 0.05 % Show Material materials with Phosphorus of 0.05 % |

Silicon | 0.1 - 0.4 % Show Material materials with Silicon of 0.1 - 0.4 % |

Sulfur | 0.035 % Show Material materials with Sulfur of 0.035 % |